Effect of Carbon Additives on the Electrochemical Performance of Li4Ti5O12/C Anodes

The Li4Ti5O12/C composites were prepared by a hydrothermal method with in situ carbon addition. The influence of the morphology and content of various carbon materials (conductive carbon black, mesoporous carbon G_157M, and carbon replicas) on the electrochemical performance of the Li4Ti5O12/C composites was investigated. The obtained composites were characterized using X-ray diffraction, scanning electron microsopy, high-resolution transmission electron microscopy, thermogravimetric analysis, Raman spectroscopy, and N2 sorption-desorption isotherms. Morphology of the Li4Ti5O12/C composites depends on the carbon matrix used, while both morphology and the amount of carbon material have a great impact on the rate capability and cycling stability of the obtained composites. At low current densities, the Li4Ti5O12/C composite with 5 wt.% G_157M exhibits the highest discharge capacity, while at high charge-discharge rates, the Li4Ti5O12/carbon black composites show the best electrochemical performance. Thus, at ~0.1C, 5C, and 18C rates, the discharge capacities of the obtained Li4Ti5O12/C composites are 175, 120, and 70 mAh/g for G_157M, 165, 126, and 78 mAh/g for carbon replicas, and 173, 128, and 93 mAh/g for carbon black. After 100 cycles, their capacity retention is no less than 95%, suggesting their promising application perspective.


Introduction
In recent years, lithium titanate with a spinel structure (Li 4 Ti 5 O 12 , LTO) has been considered as a promising anode material for high-power applications in lithium-ion batteries, such as electric vehicles and backup power systems. LTO exhibits an exceptional stability and a long lifetime cycling due to a near zero lattice volume change (<1%) during the lithium insertion-extraction process [1,2], which is 13 times less than that of graphite, widely used as an anode material in commercial lithium-ion batteries [3,4]. Compared with graphite, lithium titanate has a flat and relatively high operating potential of about 1.55 V (vs. Li/Li + ), which results in a decreased cell potential, avoiding an undesired reduction (decomposition) of most electrolyte solvents with the SEI (solid electrolyte interface) formation [2,5]. However, the main disadvantage that restricts the wide practical use of lithium titanate is its poor rate capability caused by its low electronic conductivity (−10 −13 S/cm) and lithium ion diffusion coefficient (−10 −12 cm 2 /s) [2,6].

Materials and Methods
Mesoporous carbon material G_157M (NanoTechCenter LLC, Tambov, Russia), carbon replicas (CR), prepared according to the procedure described elsewhere [49], and carbon black (CB, Timcal Graphite and Carbon, Switzerland) were used for the Li 4 Ti 5 O 12 /C composites synthesis. Carbon materials were pre-treated in concentrated nitric acid for 1 h and washed with deionized water. There are two main reasons for oxidizing the surface of carbon materials. The first was to impart the ability of carbon materials to form a colloidal solution in aqueous medium by attaching different functional groups directly to their surface. Moreover, the introduction of oxygen-containing groups onto the carbon surface was expected to facilitate the binding of carbon materials to lithium titanate. The predetermined amount of carbon in the Li 4 Ti 5 O 12 /C composites was 0, 5, or 20 wt.%. The Li 4 Ti 5 O 12 /C composites were prepared hydrothermally using a previously developed procedure [50]. Firstly, the predetermined amount of pre-treated carbon material was ultrasonically dispersed in 0.5 M LiOH solution for 15 min. Then, titanium butoxide was added dropwise in the molar ratio of Li:Ti = 3:1 under vigorous stirring. Next, the received suspension was transferred into a steel autoclave (Teflon-lined) and kept at 130 • C for 12 h. The resulting precipitate was washed with deionized water to remove LiOH excess, dried at 80 • C for 12 h in air, ground, and calcined at 400 • C for 5 h in Ar atmosphere. The predetermined amount of carbon materials in the Li 4 Ti 5 O 12 /C composites was 0, 5, or 20 wt.%. Hereinafter, the obtained composites were denoted as LTO/5%G_157M, LTO/20%CR, or LTO/5%CB, etc., indicating the carbon material used and its predetermined amount. For comparison, a pure lithium titanate without the addition of carbon material was also prepared under the same synthesis conditions. X-ray diffraction (XRD) measurements were performed using a Rigaku D/MAX 2200 diffractometer (Rigaku, Japan), Cu-K α radiation. High-resolution transmission electron microscopy (HRTEM, Jeol JEM-2100, Jeol, Japan) and scanning electron microscopy (SEM, Carl Zeiss NVision 40 station) were used to observe the morphology and particle size of the samples. The amount of carbon materials was determined by thermogravimetric analysis (TGA) using a Netzsch TG 209 thermal balance (Netzsch, Germany) in Pt crucibles in air, at a heating rate of 10 • /min. Specific surface areas were measured by N 2 sorption-desorption at −196 • C using a Sorbtometer-M specific surface area analyzer (Katakon LLC, Russia). The obtained data were analyzed using the Brunauer-Emmett-Teller (BET) model using a desorption branch in a relative pressure range of 0.05-0.25. Before measurements, the samples were degassed at 200 • C for 1 h. Raman spectra of the samples were carried out on a DXRxi Raman Imaging Microscope with excitation by a laser line of 532 nm. Fourier Transform Infrared (FTIR) spectra were recorded on a Nicolet iS5 FTIR spectrometer with a Specac Quest attachment (attenuated total reflection measurements).
Electrochemical properties of the Li 4 Ti 5 O 12 /C composites were measured in sealed three-electrode cells. Lithium foil was used as counter and reference electrodes. Working electrodes were prepared using a standard paste method. A slurry was prepared by mixing LTO or LTO/C composite (active material), a carbon black, and a polyvinylidene fluoride binder preliminary dissolved in anhydrous N-methyl pyrrolidone in the ratio 80:15:5 (wt.%). Mass loading of active material in each electrode was about 10-15 mg/cm 2 . The electrode paste was coated onto the stainless-steel gauze (current collector), pressed under 1000 kg/cm 2 , and dried at 120 • C in a vacuum. Assembly of the electrochemical cells was performed in an Ar-filled glove box. The electrolyte solution was 1 M LiPF6 in a mixture of ethylene carbonate, diethyl carbonate, and dimethyl carbonate (1:1:1 v/v). Galvanostatic charge-discharge tests were performed at different current densities in the range of 20-8000 mA/g using a ZRU 50 mA-10 V workstation (JSC NTTs Buster, Russia). Specific discharge capacity was calculated per unit weight of LTO.

Results
Raman spectra of used carbon materials are shown in Figure 1. In the Raman spectra, two intense peaks attributed to the D-and G-bands were observed at~1340 and 1600 cm −1 , respectively. In carbonaceous materials, the G-band corresponds to the vibrational mode of carbon in sp 2 hybridization (graphite), whereas the D-band indicates disorder and imperfection in the graphite structure [51,52]. However, the Raman spectra in this region cannot be fitted with only these two bands: at least four bands are necessary. Additional bands were observed at 1220 and 1530 cm −1 , which could be attributed to the vibrations of sp 3 -hybridized carbon atoms of amorphous carbon [51,52].
In the Raman spectra of the Li 4 Ti 5 O 12 /C composites, the peaks at 225, 345, 420, 680, and 745 cm −1 , assigned to the vibrations of Li-O bonds in the LiO 4 , LiO 6 polyhedra and Ti-O bonds in TiO 6 octahedra of lithium titanate [33,53] were also observed in addition to the characteristic bands of carbon materials (Figure 1d). Their intensities are significantly higher than those of the D-and G-bands of carbon materials. At the same time, the Raman spectra of carbon-coated lithium titanate show an Energies 2020, 13, 3941 4 of 15 inverse ratio of these bands' intensities [54]. Thus, in the obtained composite materials, lithium titanate particles are most likely formed on the surface, rather than inside the pores of the carbon materials.
Energies 2020, 13, x FOR PEER REVIEW 4 of 16 octahedra of lithium titanate [33,53] were also observed in addition to the characteristic bands of carbon materials (Figure 1d). Their intensities are significantly higher than those of the D-and G-bands of carbon materials. At the same time, the Raman spectra of carbon-coated lithium titanate show an inverse ratio of these bands' intensities [54]. Thus, in the obtained composite materials, lithium titanate particles are most likely formed on the surface, rather than inside the pores of the carbon materials. The data of IR spectroscopy indicate the formation of a small number of oxygen-containing groups on the surface of carbonaceous materials during their oxidation. For example, the absorption in the region of 1720-1750 cm −1 can be attributed to the >C=O-groups, as in the case of the detonation nanodiamonds [46]. IR spectra of such materials have been widely discussed in the literature [55][56][57][58][59].
The thermogravimetric analysis (TGA) in air was performed to determine the carbon content in the as-prepared composites. According to the TGA data, the real carbon content in the obtained samples was slightly less than the predetermined value (Table 1). The data of IR spectroscopy indicate the formation of a small number of oxygen-containing groups on the surface of carbonaceous materials during their oxidation. For example, the absorption in the region of 1720-1750 cm −1 can be attributed to the >C=O-groups, as in the case of the detonation nanodiamonds [46]. IR spectra of such materials have been widely discussed in the literature [55][56][57][58][59].
The thermogravimetric analysis (TGA) in air was performed to determine the carbon content in the as-prepared composites. According to the TGA data, the real carbon content in the obtained samples was slightly less than the predetermined value (Table 1).  (Figure 2). At the same time, very weak reflections of TiO 2 can also be observed for some samples. No diffraction peaks related to a graphite structure were observed, which may be due to its low content or X-ray amorphous form of carbon materials. The crystallite sizes (coherent scattering region) of the obtained samples calculated from the Scherrer formula are given in Table 1. The addition of carbon black and carbon replicas leads to a slight decrease in crystallite size, while the opposite tendency is observed when using mesoporous carbon. According to the data of experiments on low-temperature nitrogen adsorption, the BET specific surface area of the used carbon materials decreases in a series: mesoporous carbon G_157M > carbon replicas CR > carbon black CB ( Table 2). On the one hand, the use of carbon materials with a larger surface area would lead to the formation of more dispersed lithium titanate particles. On the other hand, the availability of the surface and the concentration of sorption centers on it (mainly oxygen-containing functional groups-carboxyl, carbonyl, hydroxyl) formed after treatment by nitric acid are the main factors determining the nucleation and growth of the Li 4 Ti 5 O 12 particles. The large surface area of the mesoporous carbon G_157M is primarily determined by a significant number of nanopores, the size range of which, according to the specification, is of 1-16 nm. However, it seems that the LTO particles form on the outer surface of the carbon material rather than inside its pores. Moreover, a small number of sorption centers on its surface lead to the particle growth rather than to the formation of new ones. A slight decrease in the crystallite size with an increasing G_157M content up to 20%, as well as Raman spectroscopy data, indirectly proves it. According to the N 2 adsorption-desorption measurements, the total pore volume of the as-prepared carbon replicas is 0.3 cm 3 /g (Table 2), which along with surface area, suggests the CMK-3 type of this carbon material. A larger concentration of sorption centers on the surface of carbon black and carbon replicas results in more dispersed Li 4 Ti 5 O 12 formation.  The SEM image of the Li4Ti5O12 (reference sample) shows spherical agglomerates with a diameter of about 2 μm (Figure 3a). The agglomerates consist of nanosheets with a size of 50-70 nm by 100-200 nm and a thickness of 10-15 nm. The latter value is close to the crystallite size calculated from the XRD data. TEM images of this and other materials, in some cases, show atomic layers, mainly with an interlayer distance of 0.48 nm, which corresponds to (111) lithium titanate reflection (Figure 3b).
Carbon materials' addition during the LTO synthesis leads to some changes in the morphology of the obtained Li4Ti5O12/С composites (Figure 3c-h). In the case of the LTO/5%G_157M sample, the spherical agglomerates also remain (Figure 3c). The TEM images, however, show carbon nanotubes (according to the specification, their content in the mesoporous carbon G_157M is 25-35 wt.%), nanorods and particles with irregular shape, which are the components of the mesoporous carbon material G_157M interpenetrated into the Li4Ti5O12 nanoparticles (Figure 3d). In turn, the Li4Ti5O12  The SEM image of the Li 4 Ti 5 O 12 (reference sample) shows spherical agglomerates with a diameter of about 2 µm (Figure 3a). The agglomerates consist of nanosheets with a size of 50-70 nm by 100-200 nm and a thickness of 10-15 nm. The latter value is close to the crystallite size calculated from the XRD data. TEM images of this and other materials, in some cases, show atomic layers, mainly with an interlayer distance of 0.48 nm, which corresponds to (111) lithium titanate reflection (Figure 3b). Most carbon materials exhibit charge-discharge potentials between 0 and 1 V. Therefore, their reversible electrochemical capacity in the cycling range of Li4Ti5O12 (1-3 V) is relatively low. For example, in the case of carbon replicas (CR), its value does not exceed 20 mAh/g. Therefore, the carbon material addition cannot increase the specific electrochemical capacity of the lithium titanate-based composites in this range of potentials. For all carbon materials, a significant contribution of the irreversible capacity was associated with the SEI formation [60][61][62] due to the partial electrolyte reduction in the first charge-discharge cycle.
The charge-discharge curves of the obtained Li4Ti5O12/C composites are typical for materials based on lithium titanate with a distinguished plateau at about 1.55 V (vs. Li/Li + ), indicating a two-phase process of Li4Ti5O12 ↔ Li7Ti5O12 transformation (Figure 4). In all cases, a rather high irreversible capacity can be noted in the first charge-discharge cycle, e.g., it reaches 220 mAh/g for the LTO/5%G_157M composite. From the tenth cycle, the Coulombic efficiency approaches 100% (the values of the discharge and charge capacities coincide), which suggests an industrially acceptable efficiency of these electrodes. The Li4Ti5O12 capacity usually turns out to be noticeably lower than the theoretical one (175 mAh/g), due to its rather low conductivity [2,63]. The specific capacity of Li4Ti5O12 was 164 mAh/g at a current density of 20 mA/g and decreased markedly with an increase in the cycling rate ( Figure 4). The use of the mesoporous carbon material G_157M and carbon black during the synthesis results in a significant increase in the capacity of composite materials in the entire range of current densities, e.g., at a current density of 20 mA/g, the discharge capacities of the LTO/5%G_157M and LTO/5%CB composites reach 175 and 174 mAh/g, which are close to the theoretical value. The discharged capacity of the LTO/5%CR sample remains almost at the same level as for the pure lithium titanate (165 mAh/g). Most likely, this is due to the absence of a continuous conducting network of carbon replicas, which is confirmed by electron microscopy data. At high current densities, the LTO/5%CB sample shows the best performance ( Figure 5). For example, its discharge capacity decreases by less than half at a ~18C rate (90 mAh/g, 1C = 175 mAh/g), and it is 68 mAh/g (39% of the theoretical capacity) at a ~50C rate.
A good cycling stability was observed for all samples. At each current density, 5 charge-discharge cycles were recorded, which were well reproduced. Upon returning back to a current density of 20 mA/g after 100 charge-discharge cycles at various rates, the capacity of all the studied materials decreases by no more than 5%, which indicates excellent reversible stability. Carbon materials' addition during the LTO synthesis leads to some changes in the morphology of the obtained Li 4 Ti 5 O 12 /C composites (Figure 3c-h). In the case of the LTO/5%G_157M sample, the spherical agglomerates also remain ( Figure 3c). The TEM images, however, show carbon nanotubes (according to the specification, their content in the mesoporous carbon G_157M is 25-35 wt.%), nanorods and particles with irregular shape, which are the components of the mesoporous carbon material G_157M interpenetrated into the Li 4 Ti 5 O 12 nanoparticles (Figure 3d). In turn, the Li 4 Ti 5 O 12 nanoparticles are grown on the carbon materials, indicating the strong interfacial interaction between them. It can be noted that in contrast to unmodified lithium titanate, the agglomerates of this composite remain even after ultrasonic dispersion during sample preparation for TEM.
The agglomerates of the Li 4 Ti 5 O 12 /CB composites have an irregular form, but they are composed of the same lithium titanate nanosheets (Figure 3e). Among them, there are rounded carbon black particles with a diameter of about 20-50 nm (Figure 3f).
Actually, the carbon replicas are not mesoporous materials, but are nanorods of 100-200 nm in length and 7-10 nm in diameter, formed after annealing of the sucrose sorbed in the mesoporous silica SBA-15. These dark nanorods are clearly seen among the agglomerates of the lithium titanate nanosheets (Figure 3g,h). Moreover, despite the developed surface, these nanorods are quite large and, unlike other materials, apparently do not form their own network. The difference in the morphology of the obtained composite materials is due to the influence of the carbon material morphology on the formation of Li 4 Ti 5 O 12 particles.
Most carbon materials exhibit charge-discharge potentials between 0 and 1 V. Therefore, their reversible electrochemical capacity in the cycling range of Li 4 Ti 5 O 12 (1-3 V) is relatively low. For example, in the case of carbon replicas (CR), its value does not exceed 20 mAh/g. Therefore, the carbon material addition cannot increase the specific electrochemical capacity of the lithium titanate-based composites in this range of potentials. For all carbon materials, a significant contribution of the irreversible capacity was associated with the SEI formation [60][61][62] due to the partial electrolyte reduction in the first charge-discharge cycle.
The charge-discharge curves of the obtained Li 4 Ti 5 O 12 /C composites are typical for materials based on lithium titanate with a distinguished plateau at about 1.55 V (vs. Li/Li + ), indicating a two-phase process of Li 4 Ti 5 O 12 ↔ Li 7 Ti 5 O 12 transformation (Figure 4). In all cases, a rather high irreversible capacity can be noted in the first charge-discharge cycle, e.g., it reaches 220 mAh/g for the LTO/5%G_157M composite. From the tenth cycle, the Coulombic efficiency approaches 100% (the values of the discharge and charge capacities coincide), which suggests an industrially acceptable efficiency of these electrodes. The Li 4 Ti 5 O 12 capacity usually turns out to be noticeably lower than the theoretical one (175 mAh/g), due to its rather low conductivity [2,63]. The specific capacity of Li 4 Ti 5 O 12 was 164 mAh/g at a current density of 20 mA/g and decreased markedly with an increase in the cycling rate ( Figure 4). The use of the mesoporous carbon material G_157M and carbon black during the synthesis results in a significant increase in the capacity of composite materials in the entire range of current densities, e.g., at a current density of 20 mA/g, the discharge capacities of the LTO/5%G_157M and LTO/5%CB composites reach 175 and 174 mAh/g, which are close to the theoretical value. The discharged capacity of the LTO/5%CR sample remains almost at the same level as for the pure lithium titanate (165 mAh/g). Most likely, this is due to the absence of a continuous conducting network of carbon replicas, which is confirmed by electron microscopy data. At high current densities, the LTO/5%CB sample shows the best performance ( Figure 5). For example, its discharge capacity decreases by less than half at a~18C rate (90 mAh/g, 1C = 175 mAh/g), and it is 68 mAh/g (39% of the theoretical capacity) at a~50C rate.
A good cycling stability was observed for all samples. At each current density, 5 charge-discharge cycles were recorded, which were well reproduced. Upon returning back to a current density of 20 mA/g after 100 charge-discharge cycles at various rates, the capacity of all the studied materials decreases by no more than 5%, which indicates excellent reversible stability.        [28,32,37]. The electrochemical performance of the LTO/5%CB electrode prepared in this work is very close to the maximum value at low C rates. At high C rates, it is much better than that of Li 4 Ti 5 O 12 /C composites, in which pyrolytic carbons were used as carbon sources, and some CNTs-and graphene-based composites (Table 3). Such electrochemical performance can be due to both homogeneous distribution of carbon material, which efficaciously enhances the electronic conductivity of the Li 4 Ti 5 O 12 /C composite, and its nanostructure, which shortens the Li + -ion pathway. However, only carbon material added during the synthesis of lithium titanate composite is not enough for the successful anode operation. When the electrodes were manufactured without carbon black addition (only the as-prepared samples were used in the cell fabrication), a significant deterioration in the electrochemical properties of the obtained composites was observed over the entire Energies 2020, 13, 3941 10 of 15 range of charge-discharge rates ( Figure 6). For example, at a current density of 20 mA/g, the discharge capacities of the LTO/5%G_157M and LTO/5%G_157M composites are 150 and 165 mAh/g respectively, and significantly decrease with increasing current density. It seems that a possible solution is to introduce more carbon material at the synthesis stage. However, increasing the carbon material content to 20 wt.% (to substitute 15 wt.% carbon black added during electrochemical cell assembly) did not have the expected positive effect. Thus, the addition of 20 wt.% G_157M, CR, and CB materials results in lower capacities of the obtained composites even at low charge-discharge rates. At a current density of 20 mA/g, the discharge capacities of the LTO/20%G_157M, LTO/20%CR, and LTO/20%CB composites are 140, 120, and 150 mAh/g, respectively (Figure 7). This is due to a decrease in the lithium titanate content, which is significantly more active in this potential range. Moreover, the degradation of these samples during cycling was somewhat higher. It seems that a possible solution is to introduce more carbon material at the synthesis stage. However, increasing the carbon material content to 20 wt.% (to substitute 15 wt.% carbon black added during electrochemical cell assembly) did not have the expected positive effect. Thus, the addition of 20 wt.% G_157M, CR, and CB materials results in lower capacities of the obtained composites even at low charge-discharge rates. At a current density of 20 mA/g, the discharge capacities of the LTO/20%G_157M, LTO/20%CR, and LTO/20%CB composites are 140, 120, and 150 mAh/g, respectively ( Figure 7). This is due to a decrease in the lithium titanate content, which is significantly more active in this potential range. Moreover, the degradation of these samples during cycling was somewhat higher. It seems that a possible solution is to introduce more carbon material at the synthesis stage. However, increasing the carbon material content to 20 wt.% (to substitute 15 wt.% carbon black added during electrochemical cell assembly) did not have the expected positive effect. Thus, the addition of 20 wt.% G_157M, CR, and CB materials results in lower capacities of the obtained composites even at low charge-discharge rates. At a current density of 20 mA/g, the discharge capacities of the LTO/20%G_157M, LTO/20%CR, and LTO/20%CB composites are 140, 120, and 150 mAh/g, respectively (Figure 7). This is due to a decrease in the lithium titanate content, which is significantly more active in this potential range. Moreover, the degradation of these samples during cycling was somewhat higher. A comparison of the obtained data shows that the introduction of carbon materials during the LTO synthesis has a positive effect on the electrochemical properties of the obtained composites. However, increasing the specific surface area of carbon materials does not always give better results. Morphology of the obtained samples also plays an important role. The developed inner surface of mesoporous carbon materials, even after functionalization, practically does not interact with lithium titanate and does not increase the rate of transfer processes. Even the presence of 1D carbons in the LTO/G_157M and LTO/CR composites does not have a significant effect, and the LTO/CB composites show the best performance. At the same time, the introduction of a small amount of mesoporous carbon G_157M and carbon black with a functionalized surface can significantly increase the rate capability of the obtained composites, which is very promising for the manufacture of high-power batteries.

Conclusions
A simple hydrothermal method was successfully developed to synthesize the Li4Ti5O12 composites with mesoporous carbon G_157M, carbon replicas (CR), or carbon black. Upon the introduction of carbon materials during synthesis, the morphologies of both the LTO particles and their agglomerates change. The use of carbon materials with a functionalized surface during the synthesis allows for achieving a significant increase in the rate capacity of the obtained composites, especially at high current densities. The LTO/5%CB composite exhibits the excellent rate performance with a reversible discharge capacity of 68 mAh/g (39% of the theoretical value) at −50C. Both the content of carbon material and the procedure of the cell fabrication were shown to be important. As is known, carbon black is always used in the preparation of electrodes during cell assembly. It was shown that the use of the same amount of carbon material during the synthesis instead of carbon black does not result in the same electrochemical performance. The obtained composite materials seem to be promising for use as anodes for power lithium-ion battery applications.  A comparison of the obtained data shows that the introduction of carbon materials during the LTO synthesis has a positive effect on the electrochemical properties of the obtained composites. However, increasing the specific surface area of carbon materials does not always give better results. Morphology of the obtained samples also plays an important role. The developed inner surface of mesoporous carbon materials, even after functionalization, practically does not interact with lithium titanate and does not increase the rate of transfer processes. Even the presence of 1D carbons in the LTO/G_157M and LTO/CR composites does not have a significant effect, and the LTO/CB composites show the best performance. At the same time, the introduction of a small amount of mesoporous carbon G_157M and carbon black with a functionalized surface can significantly increase the rate capability of the obtained composites, which is very promising for the manufacture of high-power batteries.

Conclusions
A simple hydrothermal method was successfully developed to synthesize the Li 4 Ti 5 O 12 composites with mesoporous carbon G_157M, carbon replicas (CR), or carbon black. Upon the introduction of carbon materials during synthesis, the morphologies of both the LTO particles and their agglomerates change. The use of carbon materials with a functionalized surface during the synthesis allows for achieving a significant increase in the rate capacity of the obtained composites, especially at high current densities. The LTO/5%CB composite exhibits the excellent rate performance with a reversible discharge capacity of 68 mAh/g (39% of the theoretical value) at −50C. Both the content of carbon material and the procedure of the cell fabrication were shown to be important. As is known, carbon black is always used in the preparation of electrodes during cell assembly. It was shown that the use of the same amount of carbon material during the synthesis instead of carbon black does not result in the same electrochemical performance. The obtained composite materials seem to be promising for use as anodes for power lithium-ion battery applications.